Architected materials that consist of periodic arrangements of nodes and struts are lightweight and can exhibit combinations of properties (such as negative Poisson ratios) that do not occur in conventional solids. Architected materials reported previously are usually constructed from identical ‘unit cells’ arranged so that they all have the same orientation. As a result, when loaded beyond the yield point, localized bands of high stress emerge, causing catastrophic collapse of the mechanical strength of the material. This ‘post-yielding collapse’ is analogous to the rapid decreases in stress associated with dislocation slip in metallic single crystals. Here we use the hardening mechanisms found in crystalline materials to develop architected materials that are robust and damage-tolerant, by mimicking the microscale structure of crystalline materials—such as grain boundaries, precipitates and phases. The crystal-inspired mesoscale structures in our architected materials are as important for their mechanical properties as are crystallographic microstructures in metallic alloys. Our approach combines the hardening principles of metallurgy and architected materials, enabling the design of materials with desired properties.
Subscribe to Journal
Get full journal access for 1 year
only $3.90 per issue
All prices are NET prices.
VAT will be added later in the checkout.
Tax calculation will be finalised during checkout.
Rent or Buy article
Get time limited or full article access on ReadCube.
All prices are NET prices.
The datasets generated and analysed during this study are available from the corresponding author on reasonable request.
Cottrell, A. Dislocations and Plastic Flow in Crystals (Clarendon Press, New York, 1953).
Argon, A. Strengthening Mechanisms in Crystal Plasticity (Oxford Univ. Press, New York, 2007).
Dimiduk, D. M., Uchic, M. D. & Parthasarathy, T. A. Size-affected single-slip behavior of pure nickel microcrystals. Acta Mater. 53, 4065–4077 (2005).
Csikor, F. F., Motz, C., Weygand, D., Zaiser, M. & Zapperi, S. Dislocation avalanches, strain bursts, and the problem of plastic forming at the micrometer scale. Science 318, 251–254 (2007).
Pham, M. S., Holdsworth, S. R., Janssens, K. G. F. & Mazza, E. Cyclic deformation response of AISI 316L at room temperature: mechanical behaviour, microstructural evolution, physically-based evolutionary constitutive modelling. Int. J. Plasticity 47, 143–164 (2013).
Imrich, P. J., Kirchlechner, C., Motz, C. & Dehm, G. Differences in deformation behavior of bicrystalline Cu micropillars containing a twin boundary or a large-angle grain boundary. Acta Mater. 73, 240–250 (2014).
Hall, E. O. The deformation and ageing of mild steel: III. Discussion of Results. Proc. Phys. Soc. B 64, 747–753 (1951).
Petch, N. J. The cleavage strength of polycrystals. J. Iron Steel Inst. 174, 25–28 (1953).
Subedi, S., Beyerlein, I. J., LeSar, R. & Rollett, A. D. Strength of nanoscale metallic multilayers. Scr. Mater. 145, 132–136 (2018).
Wegst, U. G. K., Bai, H., Saiz, E., Tomsia, A. P. & Ritchie, R. O. Bioinspired structural materials. Nat. Mater. 14, 23–36 (2015).
Barthelat, F. Architectured materials in engineering and biology: fabrication, structure, mechanics and performance. Int. Mater. Rev. 60, 413–430 (2015).
Chen, P.-Y., McKittrick, J. & Meyers, M. A. Biological materials: functional adaptations and bioinspired designs. Prog. Mater. Sci. 57, 1492–1704 (2012).
Gu, G. X., Libonati, F., Wettermark, S. D. & Buehler, M. J. Printing nature: unraveling the role of nacre’s mineral bridges. J. Mech. Behav. Biomed. Mater. 76, 135–144 (2017).
Gibson, L. J. & Ashby, M. F. Cellular Solids: Structure and Properties (Cambridge Univ. Press, Cambridge, 1997).
Schaedler, T. A. & Carter, W. B. Architected cellular materials. Annu. Rev. Mater. Res. 46, 187–210 (2016).
Schaedler, T. A. et al. Ultralight metallic microlattices. Science 334, 962–965 (2011).
Lakes, R. Foam structures with a negative Poisson’s ratio. Science 235, 1038–1040 (1987).
Andreassen, E., Lazarov, B. S. & Sigmund, O. Design of manufacturable 3D extremal elastic microstructure. Mech. Mater. 69, 1–10 (2014).
Qin, Z., Jung, G. S., Kang, M. J. & Buehler, M. J. The mechanics and design of a lightweight three-dimensional graphene assembly. Sci. Adv. 3, e1601536 (2017).
Zheng, X. et al. Multiscale metallic metamaterials. Nat. Mater. 15, 1100–1106 (2016); addendum 16, 497 (2017).
Qiu, C. et al. Influence of processing conditions on strut structure and compressive properties of cellular lattice structures fabricated by selective laser melting. Mater. Sci. Eng. A 628, 188–197 (2015); corrigendum 638, 228–231 (2015).
Maskery, I. et al. A mechanical property evaluation of graded density Al-Si10-Mg lattice structures manufactured by selective laser melting. Mater. Sci. Eng. A 670, 264–274 (2016).
Bouaziz, O., Brechet, Y. & Embury, J. D. Heterogeneous and architectured materials: a possible strategy for design of structural materials. Adv. Eng. Mater. 10, 24–36 (2008).
Li, L. L. et al. Microcompression and cyclic deformation behaviors of coaxial copper bicrystals with a single twin boundary. Scr. Mater. 69, 199–202 (2013).
Armstrong, R., Codd, I., Douthwaite, R. M. & Petch, N. J. The plastic deformation of polycrystalline aggregates. Philos. Mag. 7, 45–58 (1962).
Kimura, Y., Inoue, T., Yin, F. & Tsuzaki, K. Inverse temperature dependence of toughness in an ultrafine grain-structure steel. Science 320, 1057–1060 (2008).
Hirth, J. P. The influence of grain boundaries on mechanical properties. Metall. Trans. 3, 3047–3067 (1972).
Suresh, S. & Ritchie, R. O. Propagation of short fatigue cracks. Int. Mater. Rev. 29, 445–475 (1984).
Pham, M. S. & Holdsworth, S. R. Role of microstructural condition on fatigue damage development of AISI 316L at 20 and 300 °C. Int. J. Fatigue 51, 36–48 (2013).
Kobayashi, S., Nakamura, M., Tsurekawa, S. & Watanabe, T. Effect of grain boundary microstructure on fatigue crack propagation in austenitic stainless steel. J. Mater. Sci. 46, 4254–4260 (2011).
Pham, M.-S. & Holdsworth, S. Evolution of relationships between dislocation microstructures and internal stresses of AISI 316L during cyclic loading at 293 K and 573 K (20 °C and 300 °C). Metall. Mater. Trans. A 45, 738–751 (2014).
Reed, R. C. The Superalloys: Fundamentals and Applications Ch. 2 (Cambridge Univ. Press, Cambridge, 2006).
Orowan, E. Discussion on internal stresses. In Symp. Internal Stresses in Metals and Alloys 451–453 (Inst. of Metals, 1948).
Hirsch, P. B. & Humpreys, F. J. The deformation of single crystals of copper and copper-zinc alloys containing alumina particles - I. Macroscopic properties and workhardening theory. Proc. R. Soc. Lond. A 318, 45–72 (1970).
Porter, D. A. & Easterling, K. E. Phase Transformations in Metals and Alloys (CRC Press, Boca Raton, 2009).
Kresling, B. in Deployable Structures and Biological Morphology (eds Furuya, H. et al.) 188–195 (Internet-First Univ. Press, Ithaca, 2008).
Zhao, H. et al. Atomic-scale understanding of stress-induced phase transformation in cold-rolled Hf. Acta Mater. 131, 271–279 (2017).
Shan, S. et al. Multistable architected materials for trapping elastic strain energy. Adv. Mater. 27, 4296–4301 (2015).
Restrepo, D., Mankame, N. D. & Zavattieri, P. D. Phase transforming cellular materials. Extreme Mech. Lett. 4, 52–60 (2015).
M.-S.P. thanks A. Rollett, F. Dunne, C. Gourlay and S. Holdsworth for discussions, T. Walton and P. Hooper for fabricating some lattices, A. Piglione for providing an SEM image of γ/γ′ microstructure, and an Engineering Alloys Fellowship awarded by the Department of Materials, Imperial College London. M.-S.P. also thanks M. M. Attallah and D. M. Dimiduk for providing the original versions of Fig. 1b, f. I.T. is grateful for funding through EPSRC grants EP/P006566/1 and EP/L02513/1, and the Royal Academy of Engineering.
Nature thanks C. Niordson, N. Pugno and the other anonymous reviewer(s) for their contribution to the peer review of this work.
A patent developed on the basis of the approach proposed in this study has been filed, managed by Imperial Innovations.
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Extended data figures and tables
a, Unit cell of the fcc lattice. b, A macro-lattice cube consisting of 8 × 8 × 8 macro-unit cells. c–e, The rotation sequence to form a twin meta-grain.
Extended Data Fig. 2 Different numbers of meta-grains within the same global volume (40 mm × 40 mm × 40 mm).
a, A single meta-grain. b, c, Two twinned meta-grains, with (b) and without (c) the outer frame. d–h, Four (d), eight (e), 16 (f), 18 (g) and 27 (h) meta-grains. The locations of the boundaries are highlighted.
a–c, Materials consisting of two (a), eight (b) and 16 (c) meta-grains.
a, Stress–strain curves of architected materials consisting of different numbers of meta-grains. b, The flow stress σf of architected materials containing meta-grains at a given nominal strain of 40% increases as the size of the meta-grains decreases.
a, Model of eight meta-grains. b, c, The orientations of lattices (with respect to the global X, Y and Z co-ordinates) in the four meta-grains in the top (b) and bottom (c) layers.
Extended Data Fig. 6 Deformation behaviour of an architected material containing eight meta-grains separated by incoherent high-angle boundaries.
a, b, Macro-lattice fabricated from 316L stainless steel (a) and an elasto-plastic polymer (b). c, d, Stress–strain constitutive behaviour of the macro-lattices fabricated from the steel (c) and polymer (d).
a, Meta-precipitate lattice (orange) embedded in the matrix. b, Cubic morphology and locations of meta-precipitates inside the fcc meta-phase. c, fcc unit cell of the matrix. d, Face-centred tetragonal unit cell of the meta-precipitate.
This material contains 25 meta-precipitates.
a, Single fcc-phase meta-grain. b, Single bcc-phase meta-grain. c, A cube of meta-polygrains (left panel) consisting of two meta-phases: fcc (top and bottom layers; middle panel) and bcc (middle layer; right panel).
a, Unit cell. b, hcp-inspired meta-phase.
Red lines represent the helical movements of basal nodes; for clarity, only the movement of basal nodes on the top plane are shown.
Finite-element method simulation of an architected material containing two twinned meta-grains mimicking twinned bi-crystals. Colour represents the degrees of true strain during compression
Experimental record of the deformation behaviour of an architected hexagonal lattice during a compression loading–unloading cycle
Finite-element method simulation of the deformation behaviour of an architected hexagonal lattice during a compression loading–unloading cycle. Colour represents the degrees of true strain during deformation
About this article
Cite this article
Pham, MS., Liu, C., Todd, I. et al. Damage-tolerant architected materials inspired by crystal microstructure. Nature 565, 305–311 (2019). https://doi.org/10.1038/s41586-018-0850-3
Chinese Journal of Mechanical Engineering (2021)
Journal of Mechanical Science and Technology (2021)
Science China Technological Sciences (2021)
Acta Mechanica Solida Sinica (2021)
The International Journal of Advanced Manufacturing Technology (2021)